PULPSHEET PROPERTIES OF SODA PULP OF MIRACULOUS BERRY (THAUMATOCOCCUS DANIELLII BENTH.) STALK AS A GLOBAL FIBROUS RAW MATERIAL FOR PAPERMAKING
Sustainable global fibre supply for pulp and papermaking is becoming more important in the advent of climate change and increased demand for paper and paper products worldwide. This has resulted in alternative search for Non-Wood Fibrous(NWF) raw material to supplement existing supply. In this study, the potential of an indigenous NWF material for papermaking was carried out to determine its suitability for paper production. Fibre properties and chemical composition were carried out using Franklin’s and Tappi standard methods. An alkaline pulping process namely soda pulping method was used to pulp stalks of Thaumatococcus daniellii obtained from cocoa plantation where it was grown as undergrowth. The resulting pulp was refined in a PFI mill at three levels of revolution and evaluated for pulpsheet properties using Tappi standard methods. The fibre characteristics were generally superior to most hardwoods used for papermaking with average stalk length of 1.53mm±0.18 for young stalk and 2.02±0.26 for mature stalks. Fibre length was 2.66±0.08 and 2.71±0.06mm while Runkel ratio and flexibility on the average were 0.57 and 65% respectively. Lignin and cellulose contents had average value of 13.05% and 39.0% with cellulose:lignin ratio of 2.99. Tear index of unbeaten pulp was 2.23mN.m2/g and decreased with beating revolution. Burst index was 1.36kPa.m2/g for the unbeaten pulp and increased appreciably to 5.56kPa.m2/g. Breaking length increased from 314m for unbeaten pulp to 573m after beating at 3200 revolution. Based on the findings of this study, the pulp from Thaumatococcus daniellii meet basic requirements of acceptability and suitability for paper production.
Keywords: Non-wood fibre, fibre dimensions, papermaking potential, pulpsheet properties, Thaumatococcus daniellii
Ashori, A. (2006): Non-wood fibres- A potential source of raw material in papermaking. Polymer-Plastic Technol. Eng., 45: 1133-1136.
Atchinson, J.E. (1998): Update on global use of non-wood plant ﬁbers and some prospects for their greater use in the United States. In: Proceedings of the North American Nonwood Fiber Symposium, Atlanta, p. 1–3.
Dutt, D. and Tyagi, C.H. (2011). Comparison of various eucalyptus species for their morphological, chemical, pulp and paper making characteristics. Indian J. Chem. Technol. 18:145-151.
Dutt, D., Upadhyay, J.S., Singh, B. and Tyagi, C.H. (2009): Studies on Hibiscus cannabinus and Hibiscus sabdariffa as an alternative pulp blend for softwood: An optimization of kraft delignification process. Industrial Crops and Products 29: 16-26.
Dutt, D., Upadhyaya, J.S. and Tyagi, C.H. (2010): Studies on Hibiscus cannabinus, Hibiscus sabdariffa and Cannabinus sativa pulp to be a substitute for softwood pulp – Part 1: AS-AQ delignification process, BioResources 5: 2123-2136.
Enayati, A.A., Hamzeh, Y., Mirshokraie, S.A. and Molaii, M. (2009). Papermaking potential of Canola stalks. BioResources 4:245-256.
Fišerová, M. and Gigac, J. (2011). Comparison of hardwood kraft pulp fibre Characteristics and tensile strength. Cellulose Chem. Technol. 45:627-631.
Franklin, G.L. (1945). Preparation of thin selection of synthetic resins and wood-resins composites and a new macerating method for wood. Nature 155:3924:51
Han, J.S., Miyashita, E.S. and Spielvogel, S.J. (1999): Properties of kenaf from various cultivars, growth and pulping conditions. In: Presented at the 5th Chemical Congress of North America, The American Chemical Society, Cancun, Quintana Roo, Mexico.
Horn, R.A. (1974). Morphology of wood pulp fibre from softwoods and influence on paper strength. FPL, Forest Service USDA, 13pp.
Horn, R.A. (1978). Morphology of pulp fibre from hardwoods and influence on paper strength. Research Paper FPL 312, Forest Service USDA, 12pp
Hurter, R.W. (1997): Non-wood plant fibre characteristics. TAPPI 1997 short course notes, TAPPI, Atlanta, USA.
Hurter, R.W. and Riccio, F.A. (1998): Why CEOS don’t want to hear about non-woods. Or should they? In: Tappi Proceedings, A Nonwood Fiber Symposium, Atlanta GA, USA, pp. 1–11.
Ilvessalo-Pfaffli, M.S. (1995): Fibre atlas: identification of paper making fibres. Springer Verlag. Berling, 400p
Jimenez, L., Ramos, E., Rodriguez, A., De La Torre, M.J. and Ferrer, J.L. (2005): Optimization of Pulping conditions of abaca. An alternative raw material for producing cellulose pulp. Bioresour. Technol., 96: 977–983.
Khantayanuwong, S., Kaewmanee, S. and Shusri, A. (2006): Relationships between the changed apparent density of recycled handsheets and their mechanical and physical properties. Kasetsart J. (Nat. Sci.) 40: 541-548.
Nieschlag, H.J., Nelson, G.H., Wolff, I.A. and Pardue, R.E. (1960): A search for new fiber crops. Tappi J. 43:193–201.
O’Brien, J. (2006): Paper demand continues to grow. Paper Age, 122:1
Ogbonnaya, C.I., Roay-Macauley, H., Nwalozie, M.C. and Annerose, D.J.M. (1997): Physical and histochemical properties of kenaf (Hibiscus cannabinaus L.) grown under water deficit on a sandy soil. Ind. Crops Prod. 7: 9–18.
Ogunsile, B.O. and Uwajeh, C.F. (2009): Evaluation of the Pulp and Paper Potentials of Nigerian Grown Bambusa vulgaris, World Appl. Sci. J. 6:536-541.
Oluwadare, A.O. and Sotannde, O.A (2002): Preliminary Investigation into the Fibre Characteristics of Miraculous berry (Thaumatococcus daniellii.Benth). Agric. Sci. J. 172-79.
Oluwadare, A.O. and Sotannde, O.A. (2006): Variation of the fibre dimensions in the Stalks of Miraculous berry (Thaumatococcus daniellii Benth). Prod. Agric. Technol 2:85-90.
Omotoso, M.A. and Ogunsile, B.O. (2009): Fibre and chemical properties of some Nigerian grown Musa species for pulp production. Asian J. Mat. Sci. 1:14-21.
Pahkala, K. (2001): Non-wood plants as raw materials for pulp and paper, Agric. Food Sci. Finland. 10:101.
Pande, H. (1998). Non-wood fibres and global fibre supply. Unasylva 193:44-50.
Richtel, M. and Galbraith, K. (2008): Back at junk value, recyclables are piling up. New York Times, December, 7. Business section.
Saikia, S.N., Goswami, T. and Ali, F. (1997): Evaluation of pulp and paper making characteristics of certain fast growing plants. Wood Sci. Technol. 31: 467–475.
Sanjuan, R., Anzaldo, J., Vargas, J., Turrado, J. and Patt, R. (2001). Morphological and chemical composition of pith and fibres from Mexican sugarcane bagasse. Holzals Roh-und Werkstoff 59:447-450
Shakhes, J., Zeinaly, F., Marandi, M.A.B. and Saghafi, T. (2011a): The effects of processing variables on the soda and soda-AQ pulping of kenaf bast fibre. BioResources 6:4626-4639.
Tutus, A., Comlekcioglu, N., Karaman, S. and Alma, M.H. (2010): Chemical composition and fibre properties of Crambe orientalis and C. tataria. Int. J. Agric. Biol. 12:1814-9596.
Udohitinah, J.S. and Oluwadare, A.O. (2011): Pulping properties of Kraft Pulp of Nigerian- Grown Kenaf (Hibiscus cannabinus L.). BioResources 6:751-761.
Ververis, C., Georghiou, K., Christodoulakis, N., Santas, P. and Santas, R. (2004): Fiber dimensions, lignin and cellulose content of various plant materials and their suitability for paper production. Ind. Crops Prod. 19: 245–254.
Walia, Y.K. (2013). Chemical and physical analysis of Morus nigra (Black mulberry) for its pulpability. Asian J. of Adv. Basic Sci. 1:40-44.